View stunning SlideShares in full-screen with the new iOS app!Introducing SlideShare for AndroidExplore all your favorite topics in the SlideShare appGet the SlideShare app to Save for Later — even offline
View stunning SlideShares in full-screen with the new Android app!View stunning SlideShares in full-screen with the new iOS app!
The use of shotcrete for the support of underground excavations was pioneered by the
civil engineering industry. Reviews of the development of shotcrete technology have
been presented by Rose (1985), Morgan (1992) and Franzén (1992). Rabcewicz
(1969) was largely responsible for the introduction of the use of shotcrete for tunnel
support in the 1930s, and for the development of the New Austrian Tunnelling
Method for excavating in weak ground.
In recent years the mining industry has become a major user of shotcrete for
underground support. It can be expected to make its own contributions to this field as
it has in other areas of underground support. The simultaneous working of multiple
headings, difficulty of access and unusual loading conditions are some of the
problems which are peculiar to underground mining and which require new and
innovative applications of shotcrete technology.
An important area of shotcrete application in underground mining is in the support of
'permanent' openings such as ramps, haulages, shaft stations and crusher chambers.
Rehabilitation of conventional rockbolt and mesh support can be very disruptive and
expensive. Increasing numbers of these excavations are being shotcreted immediately
after excavation. The incorporation of steel fibre reinforcement into the shotcrete is
an important factor in this escalating use, since it minimises the labour intensive
process of mesh installation.
Recent trials and observations suggest that shotcrete can provide effective support in
mild rockburst conditions (McCreath and Kaiser, 1992, Langille and Burtney, 1992).
While the results from these studies are still too limited to permit definite conclusions
to be drawn, the indications are encouraging enough that more serious attention will
probably be paid to this application in the future.
15.2 Shotcrete technology
Shotcrete is the generic name for cement, sand and fine aggregate concretes which are
applied pneumatically and compacted dynamically under high velocity.
15.2.1 Dry mix shotcrete
As illustrated in Figure 15.1, the dry shotcrete components, which may be slightly
pre-dampened to reduce dust, are fed into a hopper with continuous agitation.
Compressed air is introduced through a rotating barrel or feed bowl to convey the
ĐƯỢC CHIA SẺ BỞI: WWW.GEOSOFTVN.COM
(Nếu thấy hữu ích hãy vote và chia sẻ nhé bạn)
SHARE BY: WWW.GEOSOFTVN.COM
(If you find useful, please vote and share other)
ACTION PAR: WWW.GEOSOFTVN.COM
(Si vous trouvez utiles, s'il vous plaît vote et d'actions, autres)
SHARE ПО: WWW.GEOSOFTVN.COM
(Если вы найдете полезную, пожалуйста, голосовать и обмениваться другой)
Shotcrete technology 277
materials in a continuous stream through the delivery hose. Water is added to the mix
at the nozzle. Gunite, a proprietary name for dry-sprayed mortar used in the early
1900's, has fallen into disuse in favour of the more general term shotcrete.
pre-dampened shotcrete mix
Figure 15.1: Simplified sketch of a typical dry mix shotcrete system.
After Mahar et al (1975).
Vacuum helps to restore pumping air and accelerator
tube to normal shape
rubber nozzle tip
wet mix shotcrete
roller rotating blades
Figure 15.2: One typical type of wet mix shotcrete machine. After Mahar et
15.2.2 Wet mix shotcrete
In this case the shotcrete components and the water are mixed (usually in a truck
mounted mixer) before delivery into a positive displacement pumping unit, which
then delivers the mix hydraulically to the nozzle where air is added to project the
material onto the rock surface.
278 Chapter 15: Shotcrete support
The final product of either the dry or wet shotcrete process is very similar. The dry
mix system tends to be more widely used in mining, because of inaccessibility for
large transit mix trucks and because it generally uses smaller and more compact
equipment. This can be moved around relatively easily in an underground mine
environment. The wet mix system is ideal for high production applications in mining
and civil engineering, where a deep shaft or long tunnel is being driven and where
access allows the application equipment and delivery trucks to operate on a more or
less continuous basis. Decisions to use the dry or wet mix shotcrete process are
usually made on a site-by-site basis.
15.2.3 Steel fibre reinforced micro silica shotcrete
Of the many developments in shotcrete technology in recent years, two of the most
significant were the introduction of silica fume, used as a cementitious admixture, and
steel fibre reinforcement.
Silica fume or micro silica is a by-product of the ferro silicon metal industry and is an
extremely fine pozzolan. Pozzolans are cementitious materials which react with the
calcium hydroxide produced during cement hydration. Silica fume, added in
quantities of 8 to 13% by weight of cement, can allow shotcrete to achieve
compressive strengths which are double or triple the value of plain shotcrete mixes.
The result is an extremely strong, impermeable and durable shotcrete. Other benefits
include reduced rebound, improved flexural strength, improved bond with the rock
mass and the ability to place layers of up to 200 mm thick in a single pass because of
the shotcrete's 'stickiness'. However, when using wet mix shotcrete, this stickiness
decreases the workability of the material and superplaticizers are required to restore
Steel fibre reinforced shotcrete was introduced in the 1970s and has since gained
world-wide acceptance as a replacement for traditional wire mesh reinforced plain
shotcrete. The main role that reinforcement plays in shotcrete is to impart ductility to
an otherwise brittle material. As pointed out earlier, rock support is only called upon
to carry significant loads once the rock surrounding an underground excavation
deforms. This means that unevenly distributed non-elastic deformations of significant
magnitude may overload and lead to failure of the support system, unless that system
has sufficient ductility to accommodate these deformations.
Typical steel fibre reinforced, silica fume shotcrete mix designs are summarised in
Table 15.1. These mixes can be used as a starting point when embarking on a
shotcrete programme, but it may be necessary to seek expert assistance to 'fine tune'
the mix designs to suit site specific requirements. For many dry mix applications it
may be advantageous to purchase pre-mixed shotcrete in bags of up to 1,500 kg
capacity, as illustrated in Figure 15.3.
Figure 15.4 shows the steel fibre types which are currently available on the north
American market. In addition to their use in shotcrete, these fibres are also widely
used in concrete floor slabs for buildings, in airport runways and in similar concrete
Wood et al (1993) have reported the results of a comprehensive comparative study in
which all of the fibres shown in Figure 15.4 were used to reinforce shotcrete samples,
which were then subjected to a range of tests. Plain and fibre reinforced silica fume
Shotcrete technology 279
shotcrete samples were prepared by shooting onto vertical panels, using both wet and
dry mix processes. The fibre reinforced samples all contained the same steel fibre
dosage of 60 kg/m3 (see Table 15.1). All the samples were cured under controlled
relative humidity conditions and all were tested seven days after shooting.
Table 15.1: Typical steel fibre reinforced silica fume shotcrete mix designs (After Wood, 1992)
Components Dry mix Wet mix
kg./m3 % dry kg./m3 % wet
Cement 420 19.0 420 18.1
Silica fume additive 50 2.2 40 1.7
Blended aggregate 1,670 75.5 1,600 68.9
Steel fibres 60 2.7 60 2.6
Accelerator 13 0.6 13 0.6
Superplasticizer - - 6 litres 0.3
Water reducer - - 2 litres 0.1
Air entraining admixture - - if required
Water controlled at nozzle 180 7.7
Total 2,213 100 2,321 100
Figure 15.3: Bagged pre-mixed
dry shotcrete components being
delivered into a hopper feeding a
screw conveyor, fitted with a pre-
dampener, which discharges into
the hopper of a shotcrete machine
280 Chapter 15: Shotcrete support
Figure 15.4. Steel fibre types available on the north American market. After
Wood et al (1993). (Note: all dimensions are in mm).
These tests showed that the addition of steel fibres to silica fume shotcrete enhances
both the compressive and flexural strength of the hardened shotcrete by up to 20%. A
significant increase in ductility was also obtained in all the tests on fibre reinforced
samples, compared with plain samples. While different fibres gave different degrees
of improvement, all of the fibres tested were found to exceed the levels of
performance commonly specified in north America (i.e. 7-day compressive strength
of 30 MPa for dry mix, 25 MPa for wet mix and 7-day flexural strength of 4 MPa).
Kompen (1989) carried out bending tests on slabs of unreinforced shotcrete and
shotcrete reinforced with ‘Dramix’1 steel fibres, shown in Figure 15.5. The shotcrete
had an unconfined compressive strength, determined from tests on cubes, of 50 MPa.
The results of these tests are reproduced in Figure 15.6. The peak strength of these
slabs increased by approximately 85% and 185% for 1.0 and 1.5 volume % of fibres,
respectively. The ductility of the fibre reinforced slabs increased by approximately 20
and 30 times for the 1.0 and 1.5 volume % of fibres, respectively.
Figure 15.5: ‘Dramix’ steel fibres used in slab
bending tests by Kompen (1989). The fibres are
glued together in bundles with a water soluble
glue to facilitate handling and homogeneous
distribution of the fibres in the shotcrete.
Manufactured by N.V. Bekaert S.A., B-8550 Zwevegem, Belgium.
Shotcrete technology 281
Figure 15.6: Load deflection curves for unreinforced and steel fibre reinforced shotcrete
slabs tested in bending. After Kompen (1989).
15.2.4 Mesh reinforced shotcrete
While steel fibre reinforced shotcrete has been widely accepted in both civil and
mining engineering, mesh reinforced shotcrete is still widely used and is preferred in
some applications. In very poor quality, loose rock masses, where adhesion of the
shotcrete to the rock surface is poor, the mesh provides a significant amount of
reinforcement, even without shotcrete. Therefore, when stabilising slopes in very
poor quality rock masses or when building bulkheads for underground fill, weldmesh
is frequently used to stabilise the surface or to provide reinforcement. In such cases,
plain shotcrete is applied later to provide additional support and to protect the mesh
Kirsten (1992, 1993) carried out a comprehensive set of laboratory bending tests
on both mesh and fibre reinforced shotcrete slabs. The load versus deflection curves,
that he obtained, were similar to those reported by Kompen, reproduced in Figure
15.6. He found that the load carrying capacity of the mesh and fibre reinforced
shotcrete samples were not significantly different, but that the mesh reinforced
samples were superior in bending with both point loads and uniformly distributed
loads. He concluded that this was due to the more favourable location of the mesh
reinforcement in the slabs subjected to bending.
Kirsten also concluded that the quality control, required to obtain a consistent
dosage and uniform distribution of fibres in shotcrete, is more easily achieved in civil
engineering than in mining applications. This is a reflection of the multiple working
headings and the difficulties of access that are common problems associated with
many mines. Under these circumstances, more reliable reinforcement will be obtained
with mesh reinforced rather than fibre reinforced shotcrete. However, in large mines,
in which many of the ‘permanent’ openings are similar to those on large civil
engineering sites, these problems of quality control should not arise.
282 Chapter 15: Shotcrete support
Chainlink mesh, used in many underground mining excavations to support loose
rock, is not usually suitable for shotcrete reinforcement. This is because penetration
of the shotcrete is inhibited by the twisted joints as illustrated in Figure 15.7. This
allows air cavities to form behind the mesh and these may allow water to enter and
cause corrosion of the mesh.
On the other hand, weldmesh, tightly pinned against the rock face as illuatrated in
Figure 15.8, is generally ideal for shotcrete applications. Typically the weldmesh
should be made from 4 mm diameter wire welded into a 100 mm x 100 mm grid. This
type of mesh is strong enough for most underground applications and the sheets are
light enough to he handled by one man.
Figure 15.7: Chainlink mesh, while
very strong and flexible, is not ideal
for shotcrete application because it is
difficult for the shotcrete to penetrate
Figure 15.8: Welded wire mesh,
firmly attached to the rock surface,
provides excellent reinforcement
Shotcrete applications 283
15.3 Shotcrete applications
The quality of the final shotcrete product is closely related to the application
procedures used. These procedures include: surface preparation, nozzling technique,
lighting, ventilation, communications, and crew training.
Shotcrete should not be applied directly to a dry, dusty or frozen rock surface. The
work area is usually sprayed with an air-water jet to remove loose rock and dust from
the surface to be shot. The damp rock will create a good surface on which to bond the
initial layer of shotcrete paste. The nozzleman commonly starts low on the wall and
moves the nozzle in small circles working his way up towards the back, or roof. Care
must be taken to avoid applying fresh materials on top of rebound or oversprayed
shotcrete. It is essential that the air supply is consistent and has sufficient capacity to
ensure the delivery of a steady stream of high velocity shotcrete to the rock face.
Shooting distances are ideally about 1 to 1.5 metres. Holding the nozzle further from
the rock face will result in a lower velocity flow of materials which leads to poor
compaction and a higher proportion of rebound.
A well-trained operator can produce excellent quality shotcrete manually, when
the work area is well-lit and well-ventilated, and when the crew members are in good
communication with each other using prescribed hand signals or voice activated FM
radio headsets. However, this is a very tiring and uncomfortable job, especially for
overhead shooting, and compact robotic systems are increasingly being used to permit
the operator to control the nozzle remotely. Typical robotic spray booms, used for
shotcrete application in underground excavations, are illustrated in Figures 15.9,
15.10 and 15.11.
Figure 15.9: A truck mounted shotcrete robot being used in a large civil engineering tunnel.
Note that the distance between the nozzle and the rock surface is approximately one metre.
284 Chapter 15: Shotcrete support
Figure 15.10: Compact trailer-mounted robot unit for remote controlled
Figure 15.11: Shotcrete operator using a remotely
controlled unit to apply shotcrete to a rock face in a
large civil engineering excavation.
Design of shotcrete support 285
Figure 15.12: Plastic pipes used to provide drainage for a
shotcrete layer applied to a rock mass with water-bearing
When shotcrete is applied to rock masses with well-defined water-bearing joints, it is
important to provide drainage through the shotcrete layer in order to relieve high
water pressures. Drain holes, fitted with plastic pipes as illustrated in Figure 15.12,
are commonly used for this purpose. Where the water inflow is not restricted to a few
specific features, a porous fibre mat can be attached to the rock surface before the
shotcrete layer is applied. When practical to do so, the water from these drains should
be collected and directed into a drainage ditch or sump.
15.4 Design of shotcrete support
The design of shotcrete support for underground excavations is a very imprecise
process. However, one observation, which is commonly made by practical engineers
with years of experience in using shotcrete underground, is that it almost always
performs better than anticipated. There are many examples (very few of which are
documented) where shotcrete has been used as a last act of desperation in an effort to
stabilise the failing rock around a tunnel and, to most people's surprise, it has worked.
The complex interaction between the failing rock mass around an underground
opening, and a layer of shotcrete of varying thickness with properties which change
as it hardens, defies most attempts at theoretical analysis. It is only in recent years,
286 Chapter 15: Shotcrete support
with the development of powerful numerical tools, that it has been possible to
contemplate realistic analyses, which will explore the possible support-interaction
behaviour of shotcrete. A clear understanding of shotcrete behaviour will require
many more years of experience in the use of and in the interpretation of the results
obtained from these programs. It is also important to recognise that shotcrete is very
seldom used alone and its use in combination with rockbolts, cablebolts, lattice
girders or steel sets further complicates the problem of analysing its contribution to
Current shotcrete support 'design' methodology relies very heavily upon rules of
thumb and precedent experience. Wickham et al (1972) related the thickness of a
shotcrete tunnel lining to their Rock Structure Rating (RSR). Bieniawski (1989) gave
recommendations on shotcrete thicknesses (in conjunction with rockbolts or steel
sets) for different Rock Mass Ratings (RMR) for a 10 m span opening. Grimstad and
Barton (1993) have published an updated relating different support systems, including
shotcrete and fibre reinforced shotcrete, to the Tunnelling Quality Index Q.
Vandewalle (1990) collected various rules of thumb from a variety of sources and
included them in his monograph.
Table 15.2 is a compilation of current shotcrete practice by the present author,
combining all of these empirical rules and adding in my own practical experience.
The reader is warned, that this table can only be used as an approximate guide when
deciding upon the type and thickness of shotcrete to be applied in a specific
application. Modifications will almost certainly be required to deal with local
variations in rock conditions and shotcrete quality.
Table 15.2: Summary of recommended shotcrete applications in underground mining, for
different rock mass conditions.
Rock mass Rock mass Support Shotcrete application
description behaviour requirements
Massive No spalling, None. None.
metamorphic or slabbing or failure.
igneous rock .
Massive Surfaces of some Sealing surface to Apply 25 mm thickness of plain
sedimentary rock. shales, siltstones, or prevent slaking. shotcrete to permanent surfaces as
Low stress claystones may soon as possible after excavation.
conditions. slake as a result of Repair shotcrete damage due to
moisture content blasting.
Massive rock with Fault gouge may be Provision of support Remove weak material to a depth
single wide fault or weak and erodible and surface sealing in equal to width of fault or shear zone
shear zone. and may cause vicinity of weak fault and grout rebar into adjacent sound
stability problems in of shear zone. rock. Weldmesh can be used if
adjacent jointed required to provide temporary rockfall
rock. support. Fill void with plain shotcrete.
Extend steel fibre reinforced shotcrete
laterally for at least width of gouge
Design of shotcrete support 287
Massive Surface slabbing, Retention of broken Apply 50 mm shotcrete over weldmesh
metamorphic or spalling and rock and control of anchored behind bolt faceplates, or
igneous rock. possible rockburst rock mass dilation. apply 50 mm of steel fibre reinforced
High stress damage. shotcrete on rock and install rockbolts
conditions. with faceplates; then apply second 25
mm shotcrete layer.
Extend shotcrete application down
sidewalls where required.
Massive Surface slabbing, Retention of broken Apply 75 mm layer of fibre reinforced
sedimentary rock. spalling and rock and control of shotcrete directly on clean rock.
High stress possible squeezing squeezing. Rockbolts or dowels are also needed
conditions. in shales and soft for additional support.
Metamorphic or Potential for wedges Provision of support Apply 50 mm of steel fibre reinforced
igneous rock with a or blocks to fall or in addition to that shotcrete to rock surfaces on which
few widely spaced slide due to gravity available from joint traces are exposed.
joints. loading. rockbolts or cables.
Sedimentary rock Potential for wedges Provision of support Apply 50 mm of steel fibre reinforced
with a few widely or blocks to fall or in addition to that shotcrete on rock surface on which
spaced bedding slide due to gravity available from discontinuity traces are exposed, with
planes and joints. loading. rockbolts or cables. particular attention to bedding plane
Low stress Bedding plane Sealing of weak traces.
conditions. exposures may bedding plane
deteriorate in time. exposures.
Jointed Combined structural Retention of broken Apply 75 mm plain shotcrete over
metamorphic or and stress controlled rock and control of weldmesh anchored behind bolt
igneous rock. failures around rock mass dilation. faceplates or apply 75 mm of steel
High stress opening boundary. fibre reinforced shotcrete on rock,
conditions. install rockbolts with faceplates and
then apply second 25 mm shotcrete
Thicker shotcrete layers may be
required at high stress concentrations.
Bedded and jointed Slabbing, spalling Control of rock mass Apply 75 mm of steel fibre reinforced
weak sedimentary and possibly failure and shotcrete to clean rock surfaces as soon
rock. squeezing. squeezing. as possible, install rockbolts, with
High stress faceplates, through shotcrete, apply
conditions. second 75 mm shotcrete layer.
Highly jointed Ravelling of small Prevention of Apply 50 mm of steel fibre reinforced
metamorphic or wedges and blocks progressive ravelling. shotcrete on clean rock surface in roof
igneous rock. defined by of excavation.
Low stress intersecting joints. Rockbolts or dowels may be needed
conditions. for additional support for large blocks.
Highly jointed and Bed separation in Control of bed Rockbolts or dowels required to
bedded sedimentary wide span separation and control bed separation.
rock. excavations and ravelling. Apply 75 mm of fibre reinforced
Low stress ravelling of bedding shotcrete to bedding plane traces
conditions. traces in inclined before bolting.
Heavily jointed Squeezing and Control of rock mass Apply 100 mm of steel fibre reinforced
igneous or 'plastic' flow of rock failure and dilation. shotcrete as soon as possible and
metamorphic rock, mass around install rockbolts, with face-plates,
conglomerates or opening. through shotcrete. Apply additional 50
cemented rockfill. mm of shotcrete if required. Extend
High stress support down sidewalls if necessary.
288 Chapter 15: Shotcrete support
Heavily jointed Squeezing and Control of rock mass Apply 50 mm of steel fibre reinforced
sedimentary rock 'plastic' flow of rock failure and dilation. shotcrete as soon as possible, install
with clay coated mass around lattice girders or light steel sets, with
surfaces. opening. Clay rich invert struts where required, then more
High stress rocks may swell. steel fibre reinforced shotcrete to cover
conditions. sets or girders. Forepoling or spiling
may be required to stabilise face ahead
of excavation. Gaps may be left in
final shotcrete to allow for movement
resulting from squeezing or swelling.
Gap should be closed once opening is
Mild rockburst Spalling, slabbing Retention of broken Apply 50 to 100 mm of shotcrete over
conditions in and mild rockbursts. rock and control of mesh or cable lacing which is firmly
massive rock failure propagation. attached to the rock surface by means
subjected to high of yielding rockbolts or cablebolts.